Direct Demonstration of a Magnetic Dead Layer Resulting ... The formation of the dead layer is...
Embed Size (px)
Transcript of Direct Demonstration of a Magnetic Dead Layer Resulting ... The formation of the dead layer is...
FU LL P
A P ER
© 2016 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim (1 of 7) 1600414wileyonlinelibrary.com
Direct Demonstration of a Magnetic Dead Layer Resulting from A-Site Cation Inhomogeneity in a (La,Sr)MnO 3 Epitaxial Film System
Lei Jin , * Chun-Lin Jia , Ionela Lindfors-Vrejoiu , Xiaoyan Zhong , Hongchu Du , and Rafal E. Dunin-Borkowski
affecting the performance of devices. [ 1–3 ] The formation of dead layers in colossal magnetoresistive manganite fi lms appears to be independent of the choice of sub- strate, although their estimated thick- nesses (which range from ≈1 to ≈10 nm) are found to depend on the substrate. [ 4–10 ]
Re 1- x Ae x MnO 3 manganites with per- ovskite structures (where Re is a triva- lent rare-earth ion and Ae is a substi- tuting divalent alkaline-earth ion) exhibit a variety of interesting properties, e.g., metal–insulator transitions, colossal magnetoresistance, and magnetocaloric behavior. [ 11–13 ] LaMnO 3 ( x = 0), one of the end compounds of the solid solu- tions, is an antiferromagnetic insulator ( T N ≈ 140 K), with orbital order induced by the cooperative Jahn–Teller (JT) effect of Mn 3+ ions below T JT ≈ 750 K. [ 14 ] With increasing Sr substitution (resulting in hole doping), La 1- x Sr x MnO 3 (0 < x < 0.6) gradually changes its room temperature behavior from that of a paramagnetic
insulator to a ferromagnetic metallic state, accompanied by a transition from an orthorhombic phase (O-phase) to a rhombo- hedral phase (R-phase) at x ≈ 0.2. [ 15–17 ]
Bulk La 0.7 Sr 0.3 MnO 3 (hereafter referred to as LSMO with x ≈ 0.3) has a rhombohedral structure with space group R-3c. [ 18 ] In the R-3c structure, MnO 6 octahedra rotate in a way that can
The degradation of the functional properties of epitaxial oxide fi lms and the performance of related devices have often been attributed to the presence of so-called interfacial “dead layers”. Extensive efforts have been made to understand the origin of such dead layers and to avoid their formation. How- ever, the results of these efforts have not been fully satisfactory, largely as a result of the complex origin of dead layers. Here, the dead layer is studied in a sample that contains hillocks of nominally La 0.7 Sr 0.3 MnO 3 (LSMO) sand- wiched between a ferroelectric PbTiO 3 fi lm and a Nb-doped SrTiO 3 substrate using aberration-corrected (scanning) transmission electron microscopy, nanobeam electron magnetic circular dichroism spectroscopy, and related techniques. The results here reveal the presence of a 5 nm thick layer in the LSMO hillocks, close to the LSMO/Nb-SrTiO 3 interface, which exhibits dis- tinct structural and physical properties. The atomic, electronic, and magnetic structures and local chemistry of the interfacial layer are determined. It is found that octahedral rotations are suppressed in ultrathin regions at the edges of the hillocks, providing evidence for a strong effect of the adjacent Nb-SrTiO 3 and PbTiO 3 . The formation of the dead layer is discussed in the light of lattice strain and valence changes of Mn ions.
In epitaxial fi lms of functional oxides, so-called “dead layers” often form near interfaces with other materials. The electrical and/or magnetic properties of such dead layers can deviate sig- nifi cantly from those of the corresponding bulk fi lms, greatly
Dr. L. Jin, Prof. C.-L. Jia, Prof. R. E. Dunin-Borkowski Peter Grünberg Institute Research Centre Jülich D-52425 Jülich , Germany E-mail: email@example.com Dr. L. Jin, Prof. C.-L. Jia, Dr. H. C. Du, Prof. R. E. Dunin-Borkowski Ernst Ruska-Centre for Microscopy and Spectroscopy with Electrons Research Centre Jülich D-52425 Jülich , Germany Prof. C.-L. Jia The School of Electronic and Information Engineering Xi’an Jiaotong University Xi’an 710049 , China
Dr. I. Lindfors-Vrejoiu II. Physics Institute University of Cologne D-50937 Cologne , Germany Prof. X. Y. Zhong Beijing National Center for Electron Microscopy Laboratory of Advanced Materials and Department of Materials Science and Engineering Tsinghua University Beijing 100084 , China Dr. H. C. Du Central Facility for Electron Microscopy (GFE) RWTH Aachen University D-52074 Aachen , Germany
Adv. Mater. Interfaces 2016, 3, 1600414
P A P ER
© 2016 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheimwileyonlinelibrary.com1600414 (2 of 7)
be described by the Glazer notation a a a . [ 19 ] Among the La 1- x Sr x MnO 3 family (hereafter referred to as (La,Sr)MnO 3 ), x = 0.3 corre- sponds to the highest Curie temperature T C of about 370 K for the paramagnetic to ferro- magnetic phase transition. [ 15–17 ] Owning to its half metallic nature [ 20 ] and to the nearly full spin-polarized state [ 21 ] of the charge carriers (holes), LSMO is often selected as the bottom electrode in thin fi lm devices [ 22–24 ] and as the active magnetic layer in magnetic tunnel junctions. [ 25 ] LSMO fi lms can be grown epi- taxially on a wide range of commercially avail- able substrates, [ 4–10 ] including SrTiO 3 (STO), (LaAlO 3 ) 0.3 (Sr 2 AlTaO 6 ) 0.7 , and NdGaO 3 .
The dead layer in LSMO thin fi lms has been widely studied. Research efforts have been made to circumvent the formation of the dead layer, as well as to restore the func- tionalities of ultrathin LSMO fi lms through interface engineering. [ 26–29 ] One example is provided by superlattices of LSMO with layers as thin as 2 unit cells that are fer- romagnetic. [ 29 ] In this system, interfacing LSMO with ferromagnetic metallic layers of orthorhombic SrRuO 3 helps to preserve the tilts of LSMO oxygen octahedra and to main- tain the ferromagnetic properties of LSMO layers that are as thin as 2 unit cells.
Nevertheless, in general the origin of the dead layer is still not clear. Deviation from chemical stoichiometry, [ 30,31 ] lattice strain [ 4 ] and interfacial structural coupling [ 10 ] have all been suggested to play an important role in its formation, through electronic modi- fi cation [ 32 ] as well as fi eld doping. [ 33–37 ] The complex origin of the dead layer usually leads to diffi culties in considering all possible contributing factors, rendering most existing studies incomplete.
Here, we present a detailed study of a dead layer in LSMO by means of transmission electron microscopy (TEM) and scan- ning TEM (STEM). We examine heterostructures consisting of hillock-like LSMO nanostructures sandwiched between a 50 nm thick ferroelectric PbTiO 3 (PTO) fi lm and a semicon- ducting Nb-doped STO (Nb-STO) substrate. The thickness of the hillock-structured LSMO layer, which was deposited using a stencil technique, [ 22,23 ] varies from the foot to the center of each hillock. This 3D hillock geometry (as shown in Figure 1 of ref. [ 23 ] ) allows different thicknesses of the fi lm to be investi- gated simultaneously. Our results reveal the presence of a dis- tinct bottom layer, which differs from the bulk-like R-phase of LSMO present in the top parts of the hillocks in terms of its atomic structure, chemical composition, and electronic and mag- netic properties and thus constitutes a dead layer. The formation of the dead layer and its infl uence on the formation of 180° fer- roelectric domains in the adjacent PTO fi lm are discussed.
Figure 1 a shows a representative STEM high-angle annular dark-fi eld (HAADF) image of a cross-section of a LSMO hillock
sandwiched between a PTO fi lm and a Nb-STO substrate. The thickness of the hillock varies from 0 at its feet to ≈40 nm at its central part, forming a wedge-like shape at each side (see LSMO in Figure 1 b). Domain walls (DWs) separating 180° ferroelectric domains are found to occur in the PTO fi lm, depending on the thickness of the LSMO hillock layer. [ 23 ]
Figure 1 b,c shows high-resolution TEM (HRTEM) images recorded from regions of the sample denoted by frames “b” and “c” of Figure 1 a, respectively, viewed along the direction of Nb-STO. A 180° DW in the PTO fi lm is marked by a ver- tical arrow in Figure 1 b. The interface between PTO and LSMO is traced by a yellow dashed line, while that to the Nb-STO is denoted by a white double-headed arrow. In Figure 1 b, the contrast of the LSMO layer looks essentially the same. The thickness of the LSMO layer in this area of the hillock foot is measured to be between 2.5 nm on the left and 5 nm on the right. In contrast, in Figure 1 c, above the interface with the sub- strate a bottom layer of the LSMO hillock fi lm (the area below the white dashed line, denoted LSMO-I), which has a uniform thickness of ≈5 nm, has slightly different contrast from that of the main part of the LSMO hillock (denoted LSMO-M, ter- minating at the PTO/LSMO interface). Figure 1 d,e shows fast Fourier transform (FFT) images obtained from corresponding areas marked by open arrows in Figure 1 c. The FFT patterns appear to be consistent with the R and R axes of LSMO, respectively (see Figure S1a, Supporting Informa- tion). In addition to the fundamental refl ection spots shown in Figure 1 d, extra spots (see arrows) are present at ( hkl ) pc ( h = k = n /2, n = odd) positions in